Cleaving plane-dependent electronic structures of transition metal
diarsenidesCleaving plane-dependent electronic structures of
transition metal diarsenides
Gyanendra Dhakal,1 M. Mofazzel Hosen,1 Wei-Chi Chiu,2 Bahadur
Singh,3 Cheng-Yi Huang,2 Klauss Dimitri,1
Baokai Wang,2 Firoza Kabir,1 Christopher Sims,1 Sabin Regmi ,1
William Neff,1 Jonathan Denlinger,4 Hsin Lin,5
Dariusz Kaczorowski ,6 Arun Bansil,2 and Madhab Neupane 1,*
1Department of Physics, University of Central Florida, Orlando,
Florida 32816, USA 2Department of Physics, Northeastern University,
Boston, Massachusetts 02115, USA
3Department of Condensed Matter Physics and Materials Science, Tata
Institute of Fundamental Research, Mumbai 400005, India 4Advanced
Light Source, Lawrence Berkeley National Laboratory, Berkeley,
California 94720, USA.
5Institute of Physics, Academia Sinica, Taipei 11529, Taiwan
6Institute of Low Temperature and Structure Research, Polish
Academy of Sciences, Okolna 2, 50-422 Wroclaw, Poland
(Received 16 January 2020; accepted 21 April 2021; published 2 June
2021)
Topological Dirac and Weyl semimetals are currently attracting
intense interest due to their exotic physical properties.
Transition metal diarsenides such as MoAs2 and WAs2 have been
reported to harbor very high magnetoresistance suggesting the
possible existence of a topological quantum state, although this
conclusion remains dubious. Here, using systematic angle-resolved
photoemission spectroscopy (ARPES) measurements and parallel
first-principles calculations, we discuss the electronic structures
of TAs2 (T = Mo, W). Two different cleavage planes of MoAs2 are
found to harbor distinctly different surface states. Our
experiments show the presence of Dirac-like dispersions on the
(001) plane, which our first-principles calculations ascribe to
trivial surface states. Our in-depth study also finds WAs2 to
possess a trivial electronic structure. Our study emphasizes the
importance of identifying the cleavage plane in low-symmetry
systems and indicates that topological semimetallic states are not
the key for generating high magnetoresistance in MoAs2 and
WAs2.
DOI: 10.1103/PhysRevResearch.3.023170
I. INTRODUCTION
Experimental discovery of a 3D topological insulator state is
widely acknowledged as a major milestone in condensed matter and
materials physics [1–5]. This discovery has spurred intense
research interest in other classes of topological mate- rials, and
exotic states such as the Dirac semimetal [6–12], Weyl semimetal
[13–19], and nodal-line semimetal [20–23] have been theoretically
proposed and experimentally realized. In Dirac semimetals,
linearly-dispersing bands cross at low energies and behave like
Dirac fermions. Since inversion and time-reversal symmetries
protect the Dirac states, their re- alization requires the material
to be centro-symmetric and nonmagnetic [24,25]. Breaking either the
inversion or the time-reversal symmetry drives a Dirac semimetal
into a Weyl semimetal. Weyl fermions evolve as low-energy
excitations at topologically protected crossing points (Weyl nodes)
between the electron and hole bands. Weyl nodes act as monopoles or
antimonopoles of Berry curvature depending on their chirality.
Pairs of nodes of opposite chiralities are separated in momen- tum
space and behave like magnetic dipoles [13,24,25]. A recent player
on the scene is a type-II Weyl semimetal, which
*
[email protected]
Published by the American Physical Society under the terms of the
Creative Commons Attribution 4.0 International license. Further
distribution of this work must maintain attribution to the
author(s) and the published article’s title, journal citation, and
DOI.
does not conserve Lorentz invariance in that its Weyl cones are
tilted and the electron- and hole-like pockets intersect at the
Fermi surface [26]. Open Fermi surfaces, anisotropic chi- ralities,
and unconventional anomalous Hall effect are among the unusual
features of type-II Weyl semimetals. Type-II Weyl fermions are
often associated with gigantic magnetoresistance [24,25]. ARPES
studies along with parallel first-principles calculations on MoTe2,
WTe2, MoP2, and WP2 [27–30] con- firm their type-II Weyl
characteristics. These advances have spurred the exploration of
type-II Weyl states in other binary compounds of Mo and W.
Transition metal diarsenides have drawn special attention due to
their high magnetoresistance and carrier density-of-states
[31].
Recent reports of topological properties and the origin of high
magnetoresistance in MoAs2 present contradictory re- sults [32–34].
A first-principles calculation finds states with nontrivial Z2
index and suggests high magnetoresistance to result from
electron-hole compensation [32]. However, an- other study reports
trivial band structures and argues that the high magnetoresistance
results from carrier motion on the Fermi surface, which is enriched
via the open-orbit topology [33]. A quantum oscillation experiment
comple- mented by first-principles calculations indicates the
existence of open-orbits in MoAs2 [34]. The need for a
comprehensive experimental and theoretical analysis of the
electronic struc- ture of MoAs2 and its sister compound WAs2 is
thus clear. A new level of understanding of the electronic
structures can also be expected through the delineation of the
termination dependence of the electronic structure that has not yet
been reported. To date, ARPES measurements have also not been
2643-1564/2021/3(2)/023170(11) 023170-1 Published by the American
Physical Society
GYANENDRA DHAKAL et al. PHYSICAL REVIEW RESEARCH 3, 023170
(2021)
FIG. 1. Crystal structure, electronic transport, and bulk band
structure of MoAs2. (a) Conventional unit cell of MoAs2. Purple and
green spheres refer to Mo and As atoms, respectively. (b)
Conventional 3D Brillouin zone of MoAs2 with high-symmetry points
labeled. Orange and green lines represent the conventional (001)
and (100) surface projection, respectively. (c) Transverse
magnetoresistance isotherms taken at different temperatures. (d)
Resistivity measured as a function of temperature in zero field
(dark red colored symbols) and in a field of 9 T applied
perpendicular to current (orange-colored symbols). (e) Bulk band
structure of MoAs2 without SOC. Linearly crossed bands are enclosed
in the red rectangles. (f) Bulk band structure of MoAs2 with
SOC.
reported on the related compound WAs2, which belongs to the same
crystal group as MoAs2 but with a stronger spin-orbit coupling
(SOC) strength.
Here we report a systematic ARPES study of TAs2
(T = Mo, W) with parallel theoretical calculations. Electronic
structure of MoAs2 is delineated in two different cleavage planes.
Both surfaces demonstrate the existence of trivial sur- face
states. Importantly, the Dirac-like dispersions seen on the (001)
surface are formed by trivial bands. We also reveal the presence of
high magnetoresistance and similar Fermi surface features on the
(001) surface of WAs2. Since MoAs2 and WAs2 both exhibit metallic
band structures at low tempera- tures with highly populated trivial
metallic surface states, our study indicates that topological
semimetallic states are not the key for generating high
magnetoresistance in these materials.
II. METHODS
A. Sample growth and characterization
The single crystals of MoAs2 and WAs2 were grown using the chemical
vapor transport method with iodine as transport- ing agent [35].
The crystals formed needlelike structures with dimensions ∼ 1 × 0.8
× 0.4 mm3. The chemical composition was proven by energy-dispersive
x-ray analysis using an FEI scanning-electron microscope equipped
with an EDAX Gen- esis XM4 spectrometer. The crystal structure was
examined at room temperature on a Kuma-Diffraction KM4 four-circle
x-
ray diffractometer equipped with a CCD camera using Mo Kα
radiation. The experiment confirmed the monoclinic crystal
structure and the lattice constants in accord with the previ- ously
reported values [35]. Electrical resistivity measurements were
performed over 2 to 300 K employing a conventional four-point ac
technique implemented in a Quantum Design PPMS platform. Electrical
contacts were made using silver epoxy paste. A perpendicular
magnetic field was applied to measure the transverse
magnetoresistance.
B. Spectroscopic surface measurements
Synchrotron-based ARPES measurements were performed at the Advanced
Light Source (ALS), Berkeley, at beamlines 4.0.3, 7.0.2, and 10.0.1
equipped with high-efficiency R8000 and R4000 electron analyzers.
The energy resolution was set to be better than 20 meV. The angular
resolution was set to be better than 0.2 for all measurements.
Samples were cleaved in situ and measured at 15 to 25 K in a vacuum
better than 10−10 Torr. They were found to be very stable and
without degradation for the typical measurement period of 20 hours.
LEED measurements for structural analysis were performed at the ALS
beamline 4.0.3 at a base pressure of better than 10−10 Torr in the
preparation chamber. Samples were cleaved in the main chamber at a
temperature of 80 K and moved to the preparation chamber for
room-temperature LEED. The sample was further characterized by Laue
diffraction.
023170-2
CLEAVING PLANE-DEPENDENT ELECTRONIC … PHYSICAL REVIEW RESEARCH 3,
023170 (2021)
FIG. 2. Electronic structure of MoAs2 in the (001) plane. (a)
Experimental Fermi surface map where high-symmetry points of the
Brillouin zone are marked. Red lines represent the constructed
Brillouin zone. The map was obtained using photon energy of 90 eV.
(b) Calculated Fermi map. (c) Dispersion measurements along the Y
--Y direction obtained at a photon energy of 98 eV. (d)
Second-derivative plot of dispersion map in (c). (e) Calculated
dispersion map along the Y --Y direction. All data were collected
at the ALS beamline 4.0.3 at a temperature of 20 K. The orange
dotted curves are guides to the eye to compare theory and
experimental plots. The blue color represents the bulk band whereas
the red color denotes the surface band in the calculations.
FIG. 3. Electronic structure of MoAs2 (100) surface. (a) Measured
Fermi surface map of the MoAs2 (100) plane. Dashed black lines
represent the constructed Brillouin zone. (b) Calculated Fermi
surface map. (c) Electronic band dispersion along the Y --Y
direction. (d) Calculated dispersion map along the Y --Y direction.
(e) Electronic band dispersion along the M-Z-M direction. Data were
collected at the ALS beamline 10.0.1 at a temperature of 15 K using
70 eV photon energy. The orange dotted curves serve as guides to
the eye to compare theory and experimental plots. Blue color
denotes surface state and red color represent the bulk state in the
calculations.
023170-3
GYANENDRA DHAKAL et al. PHYSICAL REVIEW RESEARCH 3, 023170
(2021)
FIG. 4. Transport properties and the electronic structure of WAs2
of the (001) plane. (a) Resistivity as a function of temperature
measured in zero field (dark red curve) and in a transverse field
of 9 T (orange curve). (b) Transverse magnetoresistance isotherms
measured as a function of the field at different temperatures. (c)
Bulk band structure of WAs2 without SOC. (d) Bulk band structure of
WAs2 with SOC. (e) Measured Fermi surface map of WAs2 at the photon
energy of 35 eV. (f) Energy-momentum dispersion of WAs2 along the
Y1-X -Y1 direction. (g) Energy-momentum dispersion of WAs2 along
the Y --Y direction. All data were collected at the ALS beamline
7.0.2 at a temperature of 20 K.
C. First-principles calculations
Electronic structure was calculated by using the Vi- enna ab initio
simulation package (VASP) [36] based on the density-functional
theory (DFT) [37] with the projec- tor augmented wave (PAW) method
[36,38]. We used the generalized-gradient approximation (GGA) [39]
to model exchange-correlation effects. The energy cutoff of the
plane wave basis set was 400 eV, and the size of the k mesh was 16
× 16 × 7. An effective tight-binding model Hamiltonian was obtained
by projecting first-principles results onto Wan- nier orbitals
using the VASP2WANNIER90 [40]. The Mo d and As p orbitals were
included to generate Wannier func-
tions. We calculated the surface states by using an iterative
Green’s function method with the WannierTools package [41].
III. RESULTS AND ANALYSIS
A. Crystal structure and sample characterization
MoAs2 crystallizes in a monoclinic structure in the C2/m symmetry
group (#12) with lattice parameters: a = 9.064(7) Å, b = 3.987(1)
Å, c =7.7182(9) Å, and β= 119.37(1) [31,35], see Fig. 1(a). The
conventional bulk Brillouin zone and its 2D projections onto the
(100) and (001) surfaces are shown in Fig. 1(b). The temperature
dependence of the
023170-4
FIG. 5. Experimental geometry for ARPES measurements.
electrical resistivity of MoAs2 is presented in Fig. 1(d). At 300
K, the resistivity is about 190 μ cm and decreases down to 2.6 μ cm
at 2 K. The large residual resistivity ratio (RRR = ρ300K/ρ2K ) of
79 verifies high quality of the crystal measured. As seen in Fig.
1(d), magnetic field of 9 T applied perpendicular to electric
current hardly alters ρ(T ). The transverse magnetoresistance (MR)
taken as a function of the field at various temperatures from the
range 2-200 K is presented in Fig. 1(c). At low temperatures, the
magnitude of MR is enhanced (MR = 107% at T = 2 K and μ0H = 9 T),
and thus signals the possibility of MoAs2 hosting topological
states and/or harboring electron-hole compensation. More- over, the
observed deviation of MR from the Kohler’s rule can be associated
with the behavior in a multiband system with variable carrier
densities [31]. Bulk band structure of MoAs2
without and with the inclusion of spin-orbit coupling effects is
presented in Figs. 1(e) and 1(f), respectively. The bands in the
vicinity of the Fermi level give an impression of the Dirac
dispersion in the regions enclosed in red rectangles (0.8 eV above
the Fermi level near L and 1 eV below the Fermi level near the Z
point). These Dirac-like crossings are seen to take
FIG. 7. Bulk-band structure of MoAs2 with spin-orbit coupling.
Topological invariants were calculated by artificially shifting the
Fermi level (dashed red line) to lie between bands 2 and 3.
place away from the high-symmetry points. Note that these
Dirac-like crossings are not robust against spin-orbit coupling as
gaps are opened up when spin-orbit coupling effects are included in
the computations. Our Z2 calculations on MoAs2
show that it is topologically trivial with Z2= (0;000) when the
Fermi level lies between the bands 2 and 3. It can, however,
support a weak topological state with Z2 = (0;111) if the Fermi
level is artificially placed to lie between bands 1 and 2, see
Appendix C for details.
B. Observation of trivial band structures on the (001) plane
We carried out ARPES measurements using a VUV photon source which
allows surface-sensitive measurements. Elec- tronic structures of
the MoAs2 (001) surface are presented in Fig. 2. The experimental
Fermi surface in Fig. 2(a) con- sists of multiple Fermi pockets
indicating the metallic nature of MoAs2. A bridge-like pair of
lines at the point is re- lated to the surface bands. The
experimental Fermi surface is reasonably captured by our
first-principles calculations [Fig. 2(b)], some discrepancies can
be attributed to matrix- elements effects [42,43]. We draw
orange-colored overlay plot to directly compare theory and
experiment. Figure 2(c) displays the dispersion along the Y --Y
direction. The inner linear band marked by α, which disperses
linearly does not change shape and size with photon energy, and
manifests a
FIG. 6. LEED and Laue measurements. (a) LEED pattern of cleaved
surface 1. (b) LEED pattern of cleaved surface 2. (c) Laue
diffraction pattern of natural flat surface.
023170-5
GYANENDRA DHAKAL et al. PHYSICAL REVIEW RESEARCH 3, 023170
(2021)
FIG. 8. Photon-energy dependent electronic dispersions and their
second derivative plots along the Y --Y direction on the (001)
surface in MoAs2. (a) Dispersion maps along the Y --Y direction for
different photon energies as noted on the plots. (b) Second
derivative plots corresponding to the maps presented in panel (a).
All data were collected at the ALS beamline 4.0.3. at a temperature
of 20 K.
surface-originated Dirac-like dispersion. The α-band is seen
surrounded by the electron-like band marked β, which be- comes
stronger with varying photon energy, indicating its bulk nature. In
particular, we do not see the presence of this bulk band in the
Fermi surface map measured at a photon energy of 90 eV. Figure 2(d)
shows a second-derivative plot of the map of Fig. 2(c) which
highlights the linear crossings of the bands. In Fig. 2(e), the
calculated dispersion map is presented. It reasonably captures the
main bands observed in the experiment. Our theoretical calculations
support our view
that the α is a surface band and β is a bulk band. Lower part of
the α bands are not seen as they are buried in the bulk
bands.
C. Electronic structure of the (100) plane
We now consider the surface-dependent electronic struc- ture of
MoAs2. Figure 3(a) shows that the Fermi surface map for the (100)
plane is distinctly different from that for the (001) plane
discussed in the preceding section. Approximately circular pockets
are separated by a pair of lines. Extended
FIG. 9. ARPES measured (a) Dispersion map, (b) MDCs, and (c) EDCs
along the Y --Y direction on the (001) surface. The data were taken
at 20 K with photon energy of 92 eV. The dotted lines on the MDCs
are guides to the eye.
023170-6
CLEAVING PLANE-DEPENDENT ELECTRONIC … PHYSICAL REVIEW RESEARCH 3,
023170 (2021)
Fermi map here consists of multiple Brillouin zones presents a
dumbbell shape. The rod-like feature along the -Z di- rection
corresponds to electron-like bands. The calculated Fermi surface is
presented in Fig. 3(b) and reasonably matches the experimental
Fermi surface. Our data does not resolve all the features seen in
the theoretical plot due presumably to the effects of experimental
resolution and the ARPES matrix element. Figure 3(c) shows the
dispersion along the Y --Y where multiple bands can be seen in the
vicinity of that cross the Fermi level. In Fig. 3(d), the
first-principles calculations along the -Y direction demonstrate
the surface states, which however are topologically trivial.
Similarly, in Fig. 3(e), a pair of electron pockets can be seen in
the vicinity of the Z point. A hole-like band appears at a higher
binding energy and does not touch the electron pocket, an obvious
gap can be seen. Interestingly, the gapless Dirac-like states are
not seen in Figs. 3(c) and 3(e) (see Appendix D for details).
D. Electronic structure of WAs2
WAs2 allows us to gain insight into the effects of tun- ing the
strength of spin-orbit coupling in the transition-metal diarsenides
by substituting Mo with W. Figure 4 shows the transport behavior
and the detailed electronic band structures for the (001) surface
of WAs2. The behavior of zero-field ρ(T )
and transverse MR is rather similar to that in MoAs2 [see Fig. 4(a)
and 4(b)]. However, RRR of WAs2 is as large as 200 (ρ300 K = 140
μcm, ρ2 K = 0.7 μcm), and MR measured at T = 2 K and μ0H = 9 T
reaches nearly 1200%. As can be inferred from Fig. 4(a), in a
transverse field of 9 T, the resistance increases with decreasing
temperature below about 40 K, and then forms a plateau,
characteristic of semimetals with similar concentrations of
different charge carriers. The bulk bands in WAs2 are presented in
Figs. 4(c) and 4(d). Fig- ure 4(c) shows bulk band without
spin-orbit coupling. It does not indicate the presence of gapless
Dirac-like dispersion. The inclusion of spin-orbit coupling [Fig.
4(d)] widens the gap between the linearly dispersing bands; our
calculations are consistent with a previous study [32]. The Fermi
surface of WAs2 contains multiple Fermi pockets suggesting a
metallic nature of the material. The Fermi surface shows a
dumbbell- shaped feature with the middle of its handle located at
the
point. In order to examine the Dirac state in WAs2, the disper-
sion maps were taken along the high-symmetry directions as shown in
Figs. 4(f) and 4(g). Figure 4(f) shows the dispersion along the
Y1-X -Y1 direction as consisting of hole-like bands. The dispersion
along the Y --Y direction also shows trivial bands with the band
structure dominated by the bulk bands. In contrast to MoAs2, WAs2
does not possess a surface Dirac- like dispersion in this
direction.
FIG. 10. Photon-energy-dependent electronic band dispersions along
the M-Z-M direction from the (100) surface of MoAs2. (a) Experi-
mental spectra at various indicated photon energies. (b) Second
derivative plots corresponding to the spectra of panel (a). All the
data were collected at the ALS beamline 10.0.1 at 15 K.
023170-7
GYANENDRA DHAKAL et al. PHYSICAL REVIEW RESEARCH 3, 023170
(2021)
IV. CONCLUSIONS
We have carried out a systematic ARPES study of transition-metal
diarsenides TAs2 (T = Mo, W) in con- junction with first-principles
calculations. Surface electronic structures for the (001) and (100)
surfaces are found to be quite different with both surfaces
exhibiting the presence of multiple metallic Fermi surface pockets.
Our symmetry anal- ysis of the bulk band structures shows clearly
that neither of these diarsenides supports a topological insulator
state. This, along with the fact that these compounds respect time
reversal as well as inversion symmetry, would seem to rule out
their being either an intrinsic Dirac or a Weyl semimetal even
though the band structures display some Dirac-like
linearly-dispersing features. Our study highlights the impor- tance
of identifying the cleavage plane in electronic structure studies
of low-symmetry systems.
ACKNOWLEDGMENTS
M.N. is supported by the Air Force Office of Scientific Re- search
under Award No. FA9550-17-1-0415 and the National Science
Foundation (NSF) CAREER Award No. DMR- 1847962. The work at
Northeastern University was supported by the U.S. Department of
Energy (DOE), Office of Science, Basic Energy Sciences Grant No.
DE-FG02-07ER46352, and benefited from Northeastern University’s
Advanced Scientific Computation Center (ASCC) and the NERSC
supercomput-
ing center through DOE Grant No. DE-AC02-05CH11231. H.L.
acknowledges the support by the Ministry of Science and Technology
(MOST) in Taiwan under Grant No. MOST 109-2112-M-001-014-MY3. The
work at TIFR Mumbai was supported by the Department of Atomic
Energy of the Gov- ernment of India under Project No.
12-R&D-TFR-5.10-0100. This research used resources of the
Advanced Light Source, a U.S. Department of Energy Office of
Science User Facility, under Contract No. DE-AC02-05CH11231. We
thank Sung- Kwan Mo, Eli Rotenberg, Aaron Bostwick, and Chris
Jozwiak for beamline assistance at the LBNL.
APPENDIX A: EXPERIMENTAL GEOMETRY OF THE ARPES MEASUREMENTS
The photoemission intensity (I0) obtained in ARPES mea- surements
is directly proportional to matrix element Mk
f ,i|2 which, in turn, is proportional to |φk
f |||ε.x|||φk i |2, where φk
i
and φk f are the initial and final state wave functions of
pho-
toelectrons, respectively [44]. ε and x denote the unit vector
giving the direction of the electric field of the incoming photon
and the unit position vector of electrons, respectively.
We present our experimental ARPES geometry in Fig. 5 showing that
the incoming photon beam consists of a mixture of s and p
polarization. Both the analyzer slit and the incoming photons lie
in the mirror plane defined by the analyzer slit and
FIG. 11. Experimentally measured dispersion map, MDCs, and EDCs
along the (a) M-Z-M and (b) Y --Y direction on the (100) surface of
MoAs2. Data were collected at the ALS beamline 10.0.1 at 15
K.
023170-8
CLEAVING PLANE-DEPENDENT ELECTRONIC … PHYSICAL REVIEW RESEARCH 3,
023170 (2021)
FIG. 12. Experimental Fermi surface map of WAs2 (a) from the (001)
surface of WAs2 and (b) the corresponding second-derivative plot of
the Fermi surface. The data were collected at the ALS beam- line
7.0.2 at 20 K using 35 eV photons.
the sample surface normal. In this setup ε.x must be either odd or
even to give a nonzero photo-intensity [32,45].
APPENDIX B: LEED MEASUREMENTS OF CLEAVED SURFACE OF MoAs2
In order to study the cleaved surface, we performed LEED and Laue
spectroscopy measurements which are summarized in Fig. 6. Figures
6(a) and 6(b) show two different representa- tive cleaving planes
among multiple possible cleaving planes, LEED measurements
demonstrate that MoAs2 does not have a preferred cleaving plane.
Many samples were cleaved to in- spect the preferred cleaving plane
in MoAs2 which concluded aforementioned results. Laue diffraction
pattern of natural flat surface is presented in Fig. 6(c). The lack
of preferred cleaving plane in monoclonic transition metal
diarsenides can be attributed to low crystal symmetry and absence
of van der Waals interaction.
APPENDIX C: ELECTRONIC STRUCTURES ON THE (001) SURFACE OF
MoAs2
Figure 7 presents the bulk-band structure of MoAs2. The Fermi
energy was artificially placed to lie between the bands 2 and 3.
Our Z2 calculations for this band structure yield a trivial band
structure. Figure 8 shows experimental photon-energy-dependent
ARPES spectra for MoAs2 along the Y --Y direction and their second
derivative plots. These data exhibit the presence of a gapless
Dirac-like dispersion on the (001) plane. An electron-like band in
the vicinity of the point close to the Fermi level is suppressed at
the photon energy of 92 eV. However α-band [see Fig. 2(c)] does not
disperse with photon energies indicating the surface state (see
Fig. 8). In Fig. 9, we present MDCS and EDCs of dispersion map
along the Y --Y direction which find the presence of gapless
Dirac-like dispersion.
APPENDIX D: ELECTRONIC STRUCTURES ON THE (100) SURFACE OF
WAs2
Figure 10 presents the photon-energy-dependent disper- sion maps
along the M-Z-M direction and corresponding second derivative
plots. The dispersion maps at different pho- ton energies
demonstrate the absence of gapless Dirac-like state along this
direction. MDCs and EDCs plots of dispersion maps along the M-Z-M
and M--M (see Fig. 11) further con- firm the absence of gapless
Dirac-like state on the (100) plane.
APPENDIX E: ELECTRONIC STRUCTURE OF THE (001) SURFACE OF
WAs2.
Figures 12 to 14 present electronic structures of WAs2. The Fermi
surface is seen to be quite different from that of MoAs2.
Photon-energy-dependent spectra along the Y --Y direction (see Fig.
13) indicate the presence of non-dispersive bands at the point near
the Fermi level. MDCs and EDCs along Y --Y and Y1-X -Y1 are
presented in Fig. 14 provide a clear indication of lack of Dirac
states. The dispersion maps of WAs2 are quite different from those
of MoAs2.
FIG. 13. Photon-energy-dependent spectral maps along the Y --Y
direction on the (001) surface of WAs2. Data were collected at the
ALS beamline 7.0.2. at 20 K.
023170-9
GYANENDRA DHAKAL et al. PHYSICAL REVIEW RESEARCH 3, 023170
(2021)
FIG. 14. Dispersion map, MDCs and EDCs along the (a) Y --Y
direction, and the (b) Y1-X -Y1 direction. Data were collected at
the ALS beamline 7.0.2 at 20 K using 35 eV photons.
[1] M. Z. Hasan and C. L. Kane, Colloquium: Topological insula-
tors, Rev. Mod. Phys. 82, 3045 (2010).
[2] J. E. Moore, The birth of topological insulators, Nature
(London) 464, 194 (2010).
[3] X.-L. Qi, and S.-C. Zhang, Topological insulators and super-
conductors, Rev. Mod. Phys. 83, 1057 (2011).
[4] M. Z. Hasan, S.-Y. Xu, and M. Neupane, Topological In-
sulators, topological Dirac semimetals, topological crystalline
insulators, and topological Kondo knsulators. in Topological In-
sulators: Fundamentals and Perspectives, edited by F. Ortmann, S.
Roche, and S. O. Valenzuela (John Wiley & Sons, New York,
2015).
[5] A. Bansil, H. Lin, and T. Das, Colloquium: Topological band
theory, Rev. Mod. Phys. 88, 021004 (2016).
[6] S. Murakami, Phase transition between the quantum spin Hall and
insulator phases in 3D: Emergence of a topological gapless phase,
New J. Phys. 9, 356 (2007).
[7] S. M. Young, S. Zaheer, J. C. Y. Teo, C. L. Kane, E. J. Mele,
and A. M. Rappe, Dirac Semimetal in Three Dimensions, Phys. Rev.
Lett. 108, 140405 (2012).
[8] Z. Wang, H. Weng, Q. Wu, X. Dai, and Z. Fang, Three-
dimensional Dirac semimetal and quantum transport in Cd3As2, Phys.
Rev. B 88, 125427 (2013).
[9] M. Neupane, S.-Y. Xu, R. Sankar, N. Alidoust, G. Bian, C. Liu,
I. Belopolski, T.-R. Chang, H.-T. Jeng, H. Lin, A. Bansil, F. Chou,
and M. Z. Hasan, Observation of a three-dimensional
topological Dirac semimetal phase in high-mobility Cd3As2, Nat.
Commun. 5, 3786 (2014).
[10] B.-J. Yang and N. Nagaosa, Classification of stable three-
dimensional Dirac semimetals with nontrivial topology, Nat. Commun.
5, 4898 (2014).
[11] M. Neupane, N. Alidoust, M. M. Hosen, J.-X. Zhu, K. Dimitri,
S.-Y. Xu, N. Dhakal, R. Sankar, I. Belopolski, D. S. Sanchez, T.-R.
Chang, H.-T. Jeng, K. Miyamoto, T. Okuda, H. Lin, A. Bansil, D.
Kaczorowski, F. C. Chou, M. Z. Hasan, and T. Durakiewicz,
Observation of the spin-polarized surface state in a
noncentrosymmetric superconductor BiPd, Nat. Commun. 7, 13315
(2016).
[12] S. M. Young and C. L. Kane, Dirac Semimetals in Two Dimen-
sions, Phys. Rev. Lett. 115, 126803 (2015).
[13] X. Wan, A. M. Turner, A. Vishwanath, and S. Savrasov, Topo-
logical semimetal and Fermi-arc surface states in the electronic
structure of pyrochlore iridates, Phys. Rev. B 83, 205101
(2011).
[14] S.-M. Huang, S.-Y. Xu, I. Belopolski, C.-C. Lee, G. Chang, B.
Wang, N. Alidoust, G. Bian, M. Neupane, C. Zhang, S. Jia, A.
Bansil, H. Lin, and M. Z. Hasan, A Weyl Fermion semimetal with
surface Fermi arcs in the transition metal monopnictide TaAs class,
Nat. Commun. 6, 7373 (2015).
[15] H. Weng, C. Fang, Z. Fang, B. A. Bernevig, and X. Dai, Weyl
Semimetal Phase in Noncentrosymmetric Transition- Metal
Monophosphides, Phys. Rev. X 5, 011029 (2015).
CLEAVING PLANE-DEPENDENT ELECTRONIC … PHYSICAL REVIEW RESEARCH 3,
023170 (2021)
[16] S.-Y. Xu, I. Belopolski, N. Alidoust, M. Neupane, G. Bian, C.
Zhang, R. Sankar, G. Chang, Z. Yuan, C.-C. Lee, S.-M. Huang, H.
Zheng, J. Ma, D. S. Sanchez, B. Wang, A. Bansil, F. Chou, P. P.
Shibayev, H. Lin, S. Jia et al., Discovery of a Weyl fermion
semimetal and topological Fermi arcs, Science 349, 613
(2015).
[17] B. Q. Lv, H. M. Weng, B. B. Fu, X. P. Wang, H. Miao, J. Ma, P.
Richard, X. C. Huang, L. X. Zhao, G. F. Chen, Z. Fang, X. Dai, T.
Qian, and H. Ding, Experimental Discovery of Weyl Semimetal TaAs,
Phys. Rev. X 5, 031013 (2015).
[18] I. Belopolski, S.-Y. Xu, D. S. Sanchez, G. Chang, C. Guo, M.
Neupane, H. Zheng, C.-C. Lee, S.-M. Huang, G. Bian, N. Alidoust,
T.-R. Chang, B. K. Wang, X. Zhang, A. Bansil, H.-T. Jeng, H. Lin,
S. Jia, and M. Z. Hasan, Criteria for Directly Detecting
Topological Fermi Arcs in Weyl Semimetals, Phys. Rev. Lett. 116,
066802 (2016).
[19] M. Z. Hasan, S.-Y. Xu, and G. Bian, Topological insulators,
topological superconductors and Weyl fermion semimetals: dis-
coveries, perspectives and outlooks, Phys. Scr. T164, 014001
(2015).
[20] G. Bian, T.-R. Chang, R. Sankar, S.-Y. Xu, H. Zheng, T.
Neupert, C.-K. Chiu, S.-M. Huang, G. Chang, I. Belopolski, D. S.
Sanchez, M. Neupane, N. Alidoust, C. Liu, B. K. Wang, C.-C. Lee,
H.-T. Jeng, C. Zhang, Z. Yuan, S. Jia et al. Topo- logical
nodal-line fermions in spin-orbit metal PbTaSe2, Nat. Commun. 7,
10556 (2016).
[21] M. Neupane, I. Belopolski, M. M. Hosen, D. S. Sanchez, R.
Sankar, M. Szlawska, S.-Y. Xu, K. Dimitri, N. Dhakal, P. Maldonado,
P. M. Oppeneer, D. Kaczorowski, F. C. Chou, M. Z. Hasan, and T.
Durakiewicz, Observation of topological nodal fermion semimetal
phase in ZrSiS, Phys. Rev. B 93, 201104(R) (2016).
[22] M. M. Hosen, K. Dimitri, I. Belopolski, P. Maldonado, R.
Sankar, N. Dhakal, G. Dhakal, T. Cole, P. M. Oppeneer, D.
Kaczorowski, F. Chou, M. Z. Hasan, T. Durakiewicz, and M. Neupane,
Tunability of the topological nodal-line semimetal phase in ZrSi X
-type materials (X = S, Se, Te), Phys. Rev. B 95, 161101(R)
(2017).
[23] C. Sims, M. M. Hosen, H. Aramberri, C.-Y. Huang, G. Dhakal, K.
Dimitri, F. Kabir, S. Regmi, X. Zhou, T.-R. Chang, H. Lin, D.
Kaczorowski, N. Kioussis, and M. Neupane, Termination- dependent
topological surface states in nodal-loop semimetal HfP2, Phys. Rev.
Materials 4, 054201 (2020).
[24] M. Z. Hasan, S.-Y. Xu, I. Belopolski, and S.- M. Huang, Dis-
covery of Weyl Fermion Semimetals and Topological Fermi Arc States,
Annu. Rev. Condens. Matter Phys. 8, 289 (2017).
[25] N. P. Armitage, E. J. Mele, and A. Vishwanath, Weyl and Dirac
semimetals in three-dimensional solids, Rev. Mod. Phys. 90, 015001
(2018).
[26] A. A. Soluyanov, D. Gresch, Z. Wang, Q. Wu, M. Troyer, X. Dai,
and B. A. Bernevig, Type-II Weyl semimetals, Prediction of Weyl
semimetal in orthorhombic MoTe2, Nature (London) 527, 495
(2015).
[27] Y. Sun, S.-C. Wu, M. N. Ali, C. Felser, and B. Yan, Spectro-
scopic evidence for a type II Weyl semimetallic state in MoTe2,
Phys. Rev. B 92, 161107(R) (2015).
[28] L. Huang, T. M. McCormick, M. Ochi, Z. Zhao, M.-t. Suzuki, R.
Arita, Y. Wu, D. Mou, H. Cao, J. Yan, N. Tridevi, and A. Kaminski,
Spectroscopic evidence for a type II Weyl semimetallic state in
MoTe2, Nat. Mater. 15, 1155 (2016).
[29] Y. Wu, D. X. Mou, N. H. Jo, K. W. Sun, L. Huang, S. L. Budko,
P. C. Canfield, and A. Kaminski, Observation of Fermi arcs in the
type-II Weyl semimetal candidate WTe2, Phys. Rev. B 94, 121113(R)
(2016).
[30] G. Autès, D. Gresch, M. Troyer, A. A. Soluyanov, and O. V.
Yazyev, Robust Type-II Weyl Semimetal Phase in Transition Metal
Diphosphides XP2 (X = Mo, W), Phys. Rev. Lett. 117, 066402
(2016).
[31] J. Wang, L. Li, W. You, T. Wang, C. Cao, J. Dai and Y. Li,
Magnetoresistance and robust resistivity plateau in MoAs2, Sci.
Rep. 7, 15669 (2017).
[32] J. Chen, Y.-K. Li, J. Dai, and C. Cao, Electronic structure
and topological properties of centrosymmetric MoAs2/WAs2 from first
principles, Sci. Rep. 7, 10491 (2017).
[33] R. Lou, Y. F. Xu, L.-X. Zhao, Z.-Q. Han, P.-J. Guo, M. Li,
J.-C. Wang, B.-B. Fu, Z.-H. Liu, Y.-B. Huang, P. Richard, T. Qian,
K. Liu, G.-F. Chen, H. M. Weng, H. Ding, and S.-C. Wang,
Observation of open-orbit Fermi surface topology in the extremely
large magnetoresistance semimetal MoAs2, Phys. Rev. B 96, 241106(R)
(2017).
[34] R. Singha, A. Pariari, G. K. Gupta, T. Das, and P. Mandal,
Probing the Fermi surface and magnetotransport properties of MoAs2,
Phys. Rev. B 97, 155120 (2018).
[35] J. J. Murray, J. B. Taylor, and L. Usner, Halogen transport of
molybdenum arsenides and other transition metal pnictides, J.
Cryst. Growth 15, 231 (1972).
[36] G. Kresse and D. Joubert, From ultrasoft pseudopotentials to
the projector augmented-wave method, Phys. Rev. B 59, 1758
(1999).
[37] P. Hohenberg and W. Kohn, Inhomogeneous electron gas, Phys.
Rev. 136, B864 (1964).
[38] G. Kresse and J. Furthmuller, Efficient iterative schemes for
ab initio total-energy calculations using a plane-wave basis set,
Phys. Rev. B 54, 11169 (1996).
[39] J. P. Perdew, K. Burke, and M. Ernzerhof, Generalized Gra-
dient Approximation Made Simple, Phys. Rev. Lett. 77, 3865
(1996).
[40] N. Marzari and D. Vanderbilt, Maximally localized generalized
Wannier functions for composite energy bands, Phys. Rev. B 56,
12847 (1997).
[41] Q. Wu, S. Zhang, H.-F. Song, M. Troyer, and A. A. Soluyanov,
WannierTools: An open-source software package for novel topological
materials, Comput. Phys. Commun. 224, 405 (2018).
[42] A. Bansil and M. Lindroos, Importance of Matrix Elements in
the ARPES Spectra of BISCO, Phys. Rev. Lett. 83, 5154 (1999).
[43] M. R. Scholz, J. Sanchez-Barriga, J. Braun, D. Marchenko, A.
Varykhalov, M. Lindroos, Y. J. Wang, H. Lin, A. Bansil, J. Minr, H.
Ebert, A. Volykhov, L. V. Yashina, and O. Rader, Reversal of the
Circular Dichroism in Angle-Resolved Photoemission from Bi2Te3,
Phys. Rev. Lett. 110, 216801 (2013).
[44] A. Damascelli, Z. Hussain, and Z.-X. Shen, Angle-resolved
photoemission studies of the cuprate superconductors, Rev. Mod.
Phys. 75, 473 (2003).
[45] S. Tang, C. Zhang, D. Wong, Z. Pedramrazi, H.-Z. Tsai, C. Jia,
B. Moritz, M. Claassen, H. Ryu, S. Kahn, J. Jiang, H. Yan, M.
Hashimoto, D. Lu, R. G. Moore, C.-C. Hwang, C. Hwang, Z. Hussain,
Y. Chen, M. M. Ugeda et al., Quantum spin Hall state in monolayer
1T’-WTe2, Nat. Phys. 13, 683 (2017).